Ordering of the intermetallic Fe40at%Al structure upon heating at different
Use of the synchrotron radiation for the time-resolved evaluation
Rietveld analysis for the evolution of fitting parameters to check strain tendency and
growth of ordered domains.
Ordering Kinetics evaluation of FeAl powders
N. Cinca1*, A. Isalgué2, C. Auguet2, A. Concustell1, I.G. Cano1, J. M. Guilemany1, F. Fauth3
1Centre de Projecció Tèrmica, Fac. Química, Universitat de Barcelona, Diagonal 649 E-08028,
2 Dep. Física Aplicada, Universitat Politècnica Catalunya, Pla Palau 18 E-08003, Barcelona; Spain
3CELLS - ALBA Synchrotron. 08290 Cerdanyola del Valles, Barcelona
Contact details: firstname.lastname@example.org
In this study, time resolved X-ray diffraction experiments using synchrotron X-ray radiation have been
performed to get insight on the time and temperature dependent atomic ordering of an intermetallic Fe-40Al
(at.%) ball-milled powder. The target of the present study is to gain knowledge on the rapid heating processes
occurring during Thermal Spray coating processes. Present results show that in the temperature range 400ºC -
550ºC, the evolution of the order can be followed and modelled by fitting the powder diffraction patterns
collected within the first minutes after fast heating. Reasonable refinements have been obtained by assuming the
presence of two domains corresponding to the ordered and disordered lattices. The lattice constant changes from
0.29165±3 10-5 nm in the ball-milled powder at room temperature to 0.29281± 10-4 nm in the ordered phase
after 3000s at 550ºC. The growth of the ordered phase is proposed to be a vacancy-related process with an
activation energy of 1.04 eV. Above 550ºC, the ordering kinetics appears too fast to be resolved using the few
seconds time scale of the present experiments which is in agreement to thermal spray results conditions.
Keywords: FeAl; synchrotron; ordering; x-ray; thermal spray; coating
Ordering phenomena is a key process for the proper understanding of the outstanding properties that
intermetallic compounds can offer in terms of mechanical, electrical and magnetic properties. This has been
investigated for decades in the attempt to elucidate how slight changes on crystal lattice order result in changes
on these properties [1, 2, 3].
The order-disorder transitions take place at a so-called critical ordering temperature Tc, which exists for
either first or second-order phase transitions. At temperatures above Tc, a short-range order (SRO) parameter is
defined and the atoms are prone to order over short distances only; below Tc, a long-range order (LRO)
parameter, defined by the tendency of atoms to be surrounded by unlike atoms, shows a dependency on
increasing the temperature i.e. it either decreases continuously like CuZn or drops abruptly to zero slightly above
Tc like Cu3Au .
Certain alloys possess the ordering temperature close to the melting temperature (Tm). Such alloys keep
therefore a permanently ordered structure unless a special treatment such as high deformation by ball milling or
high dose particle irradiation is applied . Representatives of this group are Ni3Al, NiAl, FeAl, TiAl; by
contrast, examples of reversibly ordering alloys, whose Tc < Tm, can be found within Cu–Pt and Cu–Au systems
. From the first category, transition metal aluminides have been mainly investigated due to their low densities
and promising high temperature oxidation resistance properties.
But how then is their degree of order affected upon fast heating up to almost the melting point followed
by rapid cooling? This concept is interesting to elucidate what happens to Thermal Spray coating processes.
These are a group of technologies where sufficient kinetic and thermal energy are imparted to the raw material
(in powder, wire or rod form) to create a confined high-energy particle stream, and propel the energetic particles
toward the substrate using a high-pressure carrier gas. The molten or partially molten particles deform on impact
with the substrate creating cohesive bonds with each other and adhesive bonds with the substrate [5, 6]; even just
kinetic energy can be transferred to the particles in the more recent less conventional Cold Gas Spray process,
inducing solid-state bonding only by suitable plastic deformation of the material .
Due to the thermal history of the powder upon spraying, which can involve particle temperatures near the
melting point of the material (specially in conventional processes) and afterwards high cooling rates upon impact
onto the substrate, partial ordering can be obtained in intermetallic coatings . The main motivation of this
study is then to evaluate how fast a disordered intermetallic powder becomes ordered due to rapid heating, in
analogy to what happens to particles in the flame. We expect to gain insight of time-temperature dependent
atomic ordering in the processes involved during the spraying, oriented to improve the final properties. Since
usual x-ray data acquisition with proper resolution takes a long time, synchrotron radiation will be used.
Nanocrystalline Fe-40Al (at.%) structures are obtained by thermal spray from a ball milled feedstock
powder as a way to enhance mechanical properties. We have produced Fe-40Al (at.%) coatings by the high
velocity oxy-fuel (HVOF) technology, obtaining good corrosion and oxidation resistance [9, 10]. Transition
metal aluminides have strong potential for replacing superalloys and stainless steels in moderate and high
temperature structural applications. FeAl-based alloys possess an outstanding high-temperature corrosion
resistance  and they have a lower density (5.56g/cm3) compared to other iron-based materials such as cast
iron and stainless steels (e.g. in heating elements, hot-gas filters, piping and tubing, exhaust manifolds, etc.).
However, some aspects such as poor room temperature ductility and toughness and mediocre creep strength, as
well as fabrication difficulties have hindered the introduction of intermetallics in many cases as industrial
structural materials . Because of all these reasons, aluminides appear particularly interesting as coatings on
more conventional higher-strength materials which are less corrosion-resistant at high temperatures.
Many works have dealt with the order-disorder transitions in the Fe-Al system in terms of structural
changes upon temperature, mainly through magnetic, calorimetric and X- ray diffraction experiments, showing
complementary results with these techniques [13, 14]. Some authors have pointed out that the strength of
ordering behavior of late transition-metal aluminides finds its origin in the atomic size effect, since the reduction
in strain energy due to atomic size misfit can be achieved by ordering. However, the validity of this size effect
has also been questioned for years .
Owing to long data acquisition, conventional laboratory X-ray sources present serious limitations for the
study of how the order parameter in thermal equilibrium varies with temperature. On the other hand, the high
intensity offered by synchrotron X-ray radiation sources coupled with modern fast timing detectors, allows
getting insight on the kinetics of time-temperature atomic ordering processes. Such techniques are being applied
for investigating the ordering transitions [16, 17, 18, 19] as well as the evaluation of several material
crystallization kinetics [20, 21, 22, 23] and other reactions [24, 25, 26, 27]. In their work on Cu3Au, Shannon et
al., studied the order-disorder transition starting from a disordered state at an initial temperature Ti above the
critical one (Ti > Tc) and then quenching into a region of the phase diagram where the equilibrium state is
ordered (Tc > Tf ), Tf standing for final temperature . By contrast, Schaefer et al., performed some time
dependent experiments for Fe-45Al (at.%) specimens by using time-differential length scale measurements after
fast heating rates and then left isothermally treated; they obtained the vacancy formation and migration
enthalpies, 1.0 ± 0.1 eV and 1.5 ± 0.2 eV respectively . The purpose of the present study is to report the
ordering process in a Fe-40Al (at.%) ball milled powder alloy upon fast heating from the room temperature
disordered state and, to evaluate the kinetics of such ordering process as well. As mentioned above, this will help
with the understanding of the ordered phase formation in thermal spraying.
2. Experimental method
A ball milled Fe-40Al (at.%) alloy powder supplied by CEA-DTEN (Grenoble) was used for this study. It
has a nominal composition of Fe–40Al–0.05Zr (at.%) +50 ppm B+1 wt%.Y2O3.
The temperature dependent and time resolved powder diffraction experiments were performed on the
BL04-MSPD beamline of the synchrotron facility ALBA located in the Barcelona area [29, 30].
The powders were enclosed into sealed quartz capillaries of 0.5 mm diameter, and the data was collected
in transmission geometry using a monochromated beam of 0.042492 nm wavelength. The set-up included a
remote controlled heated air blower (Cyberstar) allowing collecting data at the selected sample temperatures 400,
450, 500, 550, 600, 650, 700 and 750ºC after fast heating from room temperature. The hot spot of the blower,
this is the constant temperature range of the sample, is 5 mm in length and the X-ray beam was 3 x 0.7 mm2.
The time needed for the blower to go from room temperature to the selected data acquisition temperature was
about 3-5 min, also considering a non-negligible tem